LMucko/crystallography-open-database huggingface dataset:
Characterization of the (Bi5)(3+) cluster cation: Preparation of single crystals, crystal and molecular structure of Bi5 (Al Cl4)3
Krebs, B.; Mummert, M.; Brendel, C.J.; Journal of the Less-Common Metals 116 (1986) 159–168; doi:

data_1530211
_publ_section_title
;
 Characterization of the (Bi5)(3+) cluster cation: Preparation of single
 crystals, crystal and molecular structure of Bi5 (Al Cl4)3
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              159
_journal_page_last               168
_journal_volume                  116
_journal_year                    1986
_chemical_formula_sum            'Al3 Bi5 Cl12'
_chemical_name_systematic        'Bi5 (Al Cl4)3'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   11.86
_cell_length_b                   11.86
_cell_length_c                   30.1
_cell_volume                     3666.625
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Krebs_JCOMAH_1986_1273.cif
_cod_data_source_block           Al3Bi5Cl12
_cod_database_code               1530211
Crystal structures of phases I and III of cesium lithium sulfate
Kruglik, A.I.; Simonov, M.A.; Zhelezin, E.P.; Belov, N.V.; Doklady Akademii Nauk SSSR 247 (1979) 1384–1387; doi:

data_1530212
_publ_section_title
;
 Crystal structures of phases I and III of cesium lithium sulfate
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              1384
_journal_page_last               1387
_journal_volume                  247
_journal_year                    1979
_chemical_formula_sum            'Cs Li O4 S'
_chemical_name_systematic        'Cs Li (S O4)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2n 2ac'
_symmetry_space_group_name_H-M   'P c m n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.456
_cell_length_b                   5.456
_cell_length_c                   8.82
_cell_volume                     455.041
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Kruglik_DANKAS_1979_474.cif
_cod_data_source_block           Cs1Li1O4S1
_cod_original_cell_volume        455.0409
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,y,-x)'
_cod_original_formula_sum        'Cs1 Li1 O4 S1'
_cod_database_code               1530212
The crystal structure of (N H4)2 Se O4 (N H4 H Se O4)2
Kruglik, A.I.; Simonov, M.A.; Kristallografiya 22 (1977) 1082–1085; doi:

data_1530213
_publ_section_title
;
 The crystal structure of (N H4)2 Se O4 (N H4 H Se O4)2
;
_journal_name_full               Kristallografiya
_journal_page_first              1082
_journal_page_last               1085
_journal_volume                  22
_journal_year                    1977
_chemical_formula_sum            'H18 N4 O12 Se3'
_chemical_name_systematic        '(N H4)4 (Se O4) (H Se O4)2'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                113.93
_cell_angle_beta                 93.5
_cell_angle_gamma                107.63
_cell_formula_units_Z            2
_cell_length_a                   7.133
_cell_length_b                   10.37
_cell_length_c                   10.512
_cell_volume                     662.080
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Kruglik_KRISAJ_1977_342.cif
_cod_data_source_block           H18N4O12Se3
_cod_original_cell_volume        662.0795
_cod_database_code               1530213
Crystal structure of double lithium-rubidium sulfate
Kruglik, A.I.; Misjul', S.V.; Simonov, M.A.; Kristallografiya 24 (1979) 582–585; doi:

data_1530214
_publ_section_title
;
 Crystal structure of double lithium-rubidium sulfate
;
_journal_name_full               Kristallografiya
_journal_page_first              582
_journal_page_last               585
_journal_volume                  24
_journal_year                    1979
_chemical_formula_sum            'Li O4 Rb S'
_chemical_name_systematic        'Li Rb (S O4)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2n'
_symmetry_space_group_name_H-M   'P 1 1 21/n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                89.53
_cell_formula_units_Z            4
_cell_length_a                   9.118
_cell_length_b                   5.294
_cell_length_c                   8.738
_cell_volume                     421.775
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Kruglik_KRISAJ_1979_418.cif
_cod_data_source_block           Li1O4Rb1S1
_cod_original_cell_volume        421.7751
_cod_original_sg_symbol_Hall     '-P 2ybc (z,x-z,y)'
_cod_original_formula_sum        'Li1 O4 Rb1 S1'
_cod_database_code               1530214
Crystal structure of alpha-K Er (P O3)4
Krutik, V.M.; Pobedimskaya, E.A.; Pushcharovskii, D.Yu.; Belov, N.V.; Doklady Akademii Nauk SSSR 252 (1980) 607–610; doi:

data_1530215
_publ_section_title
;
 Crystal structure of alpha-K Er (P O3)4
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              607
_journal_page_last               610
_journal_volume                  252
_journal_year                    1980
_chemical_formula_sum            'Er K O12 P4'
_chemical_name_systematic        'K Er (P O3)4'
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2c'
_symmetry_space_group_name_H-M   'P 1 1 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                91.96
_cell_formula_units_Z            2
_cell_length_a                   7.285
_cell_length_b                   8.012
_cell_length_c                   8.444
_cell_volume                     492.566
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Krutik_DANKAS_1980_563.cif
_cod_data_source_block           Er1K1O12P4
_cod_original_cell_volume        492.5662
_cod_original_sg_symbol_Hall     'P 2yb (z,x,y)'
_cod_original_formula_sum        'Er1 K1 O12 P4'
_cod_database_code               1530215
Crystal structure of arrojadite
Krutik, V.M.; Pushcharovskii, D.Yu.; Pobedimskaya, E.A.; Belov, N.V.; Kristallografiya 24 (1979) 743–750; doi:

data_1530216
_publ_section_title
;
 Crystal structure of arrojadite
;
_journal_name_full               Kristallografiya
_journal_page_first              743
_journal_page_last               750
_journal_volume                  24
_journal_year                    1979
_chemical_formula_sum
'Al0.5 Ba0.0835 Ca0.75 F1.16 Fe4.42 K0.125 Li0.25 Mg0.25 Mn1.42 Na1.13 O23.82 P6 Pb0.0835 Sr0.0835 Zn0.42'
_chemical_name_systematic
;
Na1.13 K0.125 (Ba Sr Pb)0.0835 Ca0.75 Fe4.42 Mn1.42 (Li Mg)0.25 Zn0.42 Al0.5 
(P6 O23.82 F1.16)
;
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-B 2b'
_symmetry_space_group_name_H-M   'B 1 1 2/b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                105.79
_cell_formula_units_Z            8
_cell_length_a                   16.476
_cell_length_b                   24.581
_cell_length_c                   9.996
_cell_volume                     3895.583
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Krutik_KRISAJ_1979_875.cif
_cod_data_source_block
Al0.5Ba0.0835Ca0.75F1.16Fe4.42K0.125Li0.25Mg0.25Mn1.42Na1.13O23.82P6Pb0.0835Sr0.0835Zn0.42
_cod_original_sg_symbol_Hall     '-C 2yc (-x,z,y)'
_cod_original_formula_sum
;
Al0.5 Ba0.0835 Ca0.75 F1.16 Fe4.42 K0.125 Li0.25 Mg0.25 Mn1.42 Na1.13 O23.82 
P6 Pb0.0835 Sr0.0835 Zn0.42
;
_cod_database_code               1530216
Ueber das System Li1-y Mn Ru1-x Tix O4
Krutzsch, B.; Kemmler-Sack, S.; Journal of the Less-Common Metals 124 (1986) 111–123; doi:

data_1530217
_publ_section_title
;
 Ueber das System Li1-y Mn Ru1-x Tix O4
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              111
_journal_page_last               123
_journal_volume                  124
_journal_year                    1986
_chemical_formula_sum            'Li Mn O4 Ru0.5 Ti0.5'
_chemical_name_systematic        '(Li.95 Ti.05) (Li.05 Mn Ru.5 Ti.45) O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.315
_cell_length_b                   8.315
_cell_length_c                   8.315
_cell_volume                     574.893
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Krutzsch_JCOMAH_1986_1328.cif
_cod_data_source_block           Li1Mn1O4Ru0.5Ti0.5
_cod_original_cell_volume        574.8926
_cod_original_formula_sum        'Li1 Mn1 O4 Ru0.5 Ti0.5'
_cod_database_code               1530217
Ueber das System Li1-y Mn Ru1-x Tix O4
Krutzsch, B.; Kemmler-Sack, S.; Journal of the Less-Common Metals 124 (1986) 141–147; doi:

data_1530218
_publ_section_title
;
 Ueber das System Li1-y Mn Ru1-x Tix O4
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              141
_journal_page_last               147
_journal_volume                  124
_journal_year                    1986
_chemical_formula_sum            'Li1.67 Mn O4 Ru'
_chemical_name_systematic        'Li1.67 (Mn Ru) O4'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  'I 4bw 2bw -1bw'
_symmetry_space_group_name_H-M   'I 41/a m d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.198
_cell_length_b                   8.198
_cell_length_c                   8.786
_cell_volume                     590.482
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Krutzsch_JCOMAH_1986_1329.cif
_cod_data_source_block           Li1.67Mn1O4Ru1
_cod_original_cell_volume        590.4825
_cod_original_sg_symbol_Hall     '-I 4bd 2 (x+1/2,y+1/4,z+1/8)'
_cod_original_formula_sum        'Li1.67 Mn1 O4 Ru1'
_cod_database_code               1530218
Ueber das System Li1-y Mn Ru1-x Tix O4
Krutzsch, B.; Kemmler-Sack, S.; Journal of the Less-Common Metals 124 (1986) 155–164; doi:

data_1530219
_publ_section_title
;
 Ueber das System Li1-y Mn Ru1-x Tix O4
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              155
_journal_page_last               164
_journal_volume                  124
_journal_year                    1986
_chemical_formula_sum            'Cu0.5 Li0.5 Mn O4 Ru'
_chemical_name_systematic        '(Li.5 Cu.5) (Mn Ru) O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.348
_cell_length_b                   8.348
_cell_length_c                   8.348
_cell_volume                     581.765
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Krutzsch_JCOMAH_1986_1330.cif
_cod_data_source_block           Cu0.5Li0.5Mn1O4Ru1
_cod_original_cell_volume        581.7645
_cod_original_formula_sum        'Cu0.5 Li0.5 Mn1 O4 Ru1'
_cod_database_code               1530219
Ueber das System Li1-y Mn Ru1-x Tix O4
Krutzsch, B.; Kemmler-Sack, S.; Journal of the Less-Common Metals 124 (1986) 155–164; doi:

data_1530220
_publ_section_title
;
 Ueber das System Li1-y Mn Ru1-x Tix O4
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              155
_journal_page_last               164
_journal_volume                  124
_journal_year                    1986
_chemical_formula_sum            'Cu0.5 Li0.22 Mn O4 Ru'
_chemical_name_systematic        '(Li.22 Cu.5) (Mn Ru) O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.312
_cell_length_b                   8.312
_cell_length_c                   8.312
_cell_volume                     574.271
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Krutzsch_JCOMAH_1986_1331.cif
_cod_data_source_block           Cu0.5Li0.22Mn1O4Ru1
_cod_original_cell_volume        574.2707
_cod_original_formula_sum        'Cu0.5 Li0.22 Mn1 O4 Ru1'
_cod_database_code               1530220
Spinelle im System Li1-Z Cuz Rh Ru1-x Mnx O4
Krutzsch, B.; Kemmler-Sack, S.; Journal of the Less-Common Metals 132 (1987) 37–42; doi:

data_1530221
_publ_section_title
;
 Spinelle im System Li1-Z Cuz Rh Ru1-x Mnx O4
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              37
_journal_page_last               42
_journal_volume                  132
_journal_year                    1987
_chemical_formula_sum            'Li O4 Rh Ru'
_chemical_name_systematic        'Li (Rh Ru) O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.425
_cell_length_b                   8.425
_cell_length_c                   8.425
_cell_volume                     598.012
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Krutzsch_JCOMAH_1987_1467.cif
_cod_data_source_block           Li1O4Rh1Ru1
_cod_original_cell_volume        598.0118
_cod_original_formula_sum        'Li1 O4 Rh1 Ru1'
_cod_database_code               1530221
Spinelle im System Li1-Z Cuz Rh Ru1-x Mnx O4
Krutzsch, B.; Kemmler-Sack, S.; Journal of the Less-Common Metals 132 (1987) 37–42; doi:

data_1530222
_publ_section_title
;
 Spinelle im System Li1-Z Cuz Rh Ru1-x Mnx O4
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              37
_journal_page_last               42
_journal_volume                  132
_journal_year                    1987
_chemical_formula_sum            'Cu0.5 Li0.5 O4 Rh Ru'
_chemical_name_systematic        '(Li.5 Cu.5) (Rh Ru) O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.436
_cell_length_b                   8.436
_cell_length_c                   8.436
_cell_volume                     600.357
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Krutzsch_JCOMAH_1987_1468.cif
_cod_data_source_block           Cu0.5Li0.5O4Rh1Ru1
_cod_original_cell_volume        600.3572
_cod_original_formula_sum        'Cu0.5 Li0.5 O4 Rh1 Ru1'
_cod_database_code               1530222
Synthesis of crystals, polymorphism and determination of the structure of the monoclinic form of the double molybdate K5 In (Mo O4)4
Kudin, O.V.; Efremov, V.A.; Velikodnyi, Yu.A.; Trunov, V.K.; Zhurnal Neorganicheskoi Khimii 26 (1981) 2734–2739; doi:

data_1530223
_publ_section_title
;
 Synthesis of crystals, polymorphism and determination of the structure of
 the monoclinic form of the double molybdate K5 In (Mo O4)4
;
_journal_name_full               'Zhurnal Neorganicheskoi Khimii'
_journal_page_first              2734
_journal_page_last               2739
_journal_volume                  26
_journal_year                    1981
_chemical_formula_sum            'In K5 Mo4 O16'
_chemical_name_systematic        'K5 In (Mo O4)4'
_space_group_IT_number           9
_symmetry_space_group_name_Hall  'A -2ya'
_symmetry_space_group_name_H-M   'A 1 a 1'
_cell_angle_alpha                90
_cell_angle_beta                 114.02
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.46
_cell_length_b                   12.092
_cell_length_c                   14.625
_cell_volume                     1689.617
_citation_journal_id_ASTM        ZNOKAQ
_cod_data_source_file            Kudin_ZNOKAQ_1981_884.cif
_cod_data_source_block           In1K5Mo4O16
_cod_original_sg_symbol_Hall     'C -2yc (z,y,-x)'
_cod_original_formula_sum        'In1 K5 Mo4 O16'
_cod_database_code               1530223
Atomic structure of a 4H Ga Se polytype named delta-type
Kuhn, A.; Chevalier, R.; Rimsky, A.; Acta Crystallographica B (24,1968-38,1982) 31 (1975) 2841–2842; doi:

data_2106698
_publ_section_title
;
 Atomic structure of a 4H Ga Se polytype named delta-type
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2841
_journal_page_last               2842
_journal_volume                  31
_journal_year                    1975
_chemical_formula_sum            'Ga Se'
_space_group_IT_number           186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            8
_cell_length_a                   3.755
_cell_length_b                   3.755
_cell_length_c                   31.99
_cell_volume                     390.629
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Kuhn_ACBCAR_1975_228.cif
_cod_data_source_block           Ga1Se1
_cod_original_cell_volume        390.6293
_cod_original_formula_sum        'Ga1 Se1'
_cod_database_code               2106698
Structure and hydrogen ordering in ices VI, VII, and VIII by neutron powder diffraction
Kuhs, W.F.; Finney, J.L.; Vettier, C.; Bliss, D.V.; Journal of Chemical Physics 81 (1984) 3612–3623; doi:

data_1530224
_publ_section_title
;
 Structure and hydrogen ordering in ices VI, VII, and VIII by neutron
 powder diffraction
;
_journal_name_full               'Journal of Chemical Physics'
_journal_page_first              3612
_journal_page_last               3623
_journal_volume                  81
_journal_year                    1984
_chemical_formula_sum            'D2 O'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   4.656
_cell_length_b                   4.656
_cell_length_c                   6.775
_cell_volume                     146.871
_citation_journal_id_ASTM        JCPSA6
_cod_data_source_file            Kuhs_JCPSA6_1984_1107.cif
_cod_data_source_block           D2O1
_cod_original_cell_volume        146.8707
_cod_original_formula_sum        'D2 O1'
_cod_database_code               1530224
Roentgenostructural investigation of the monohydrates of potassium trichlorineammoniaplatinate and potassium tribromineammoniaplatinate
Kukina, G.A.; Bokii, G.B.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 6 (1965) 233–243; doi:

data_1530225
_publ_section_title
;
 Roentgenostructural investigation of the monohydrates of potassium
 trichlorineammoniaplatinate and potassium tribromineammoniaplatinate
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              233
_journal_page_last               243
_journal_volume                  6
_journal_year                    1965
_chemical_formula_sum            'Br3 H5 K N O Pt'
_chemical_name_systematic        'K (Pt (N H3) Br3) (H2 O)'
_space_group_IT_number           60
_symmetry_space_group_name_Hall  '-P 2ac 2b'
_symmetry_space_group_name_H-M   'P b n a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            12
_cell_length_a                   21.524
_cell_length_b                   8.345
_cell_length_c                   14.42
_cell_volume                     2590.088
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Kukina_ZSTKAI_1965_253.cif
_cod_data_source_block           H5Br3K1N1O1Pt1
_cod_original_cell_volume        2590.089
_cod_original_sg_symbol_Hall     '-P 2n 2ab (y,z,x)'
_cod_original_formula_sum        'H5 Br3 K1 N1 O1 Pt1'
_cod_database_code               1530225
Roentgenostructural investigation of monohydrates potassium trichlorineammoniaplatinate and potassium tribromineammoniaplatinate
Kukina, G.A.; Bokii, G.B.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 6 (1965) 233–243; doi:

data_1530226
_publ_section_title
;
 Roentgenostructural investigation of monohydrates potassium
 trichlorineammoniaplatinate and potassium tribromineammoniaplatinate
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              233
_journal_page_last               243
_journal_volume                  6
_journal_year                    1965
_chemical_formula_sum            'Cl3 H5 K N O Pt'
_chemical_name_systematic        'K (Pt N H3 Cl3) (H2 O)'
_space_group_IT_number           60
_symmetry_space_group_name_Hall  '-P 2ac 2b'
_symmetry_space_group_name_H-M   'P b n a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            12
_cell_length_a                   21.048
_cell_length_b                   8.123
_cell_length_c                   13.55
_cell_volume                     2316.683
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Kukina_ZSTKAI_1965_261.cif
_cod_data_source_block           H5Cl3K1N1O1Pt1
_cod_original_sg_symbol_Hall     '-P 2n 2ab (y,z,x)'
_cod_original_formula_sum        'H5 Cl3 K1 N1 O1 Pt1'
_cod_database_code               1530226
Topochemical reactions of Lix Nb O2
Kumada, N.; Muramatu, S.; Kikkawa, S.; Muto, F.; Kinomura, N.; Koizumi, M.; Journal of Solid State Chemistry 73 (1988) 33–39; doi:

data_1530227
_publ_section_title
;
 Topochemical reactions of Lix Nb O2
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              33
_journal_page_last               39
_journal_volume                  73
_journal_year                    1988
_chemical_formula_sum            'Li0.58 Nb O2'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   2.912
_cell_length_b                   2.912
_cell_length_c                   10.46
_cell_volume                     76.815
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Kumada_JSSCBI_1988_1601.cif
_cod_data_source_block           Li0.58Nb1O2
_cod_original_cell_volume        76.81483
_cod_original_formula_sum        'Li0.58 Nb1 O2'
_cod_database_code               1530227